LMucko/crystallography-open-database huggingface dataset:
Thermodynamics and kinetics of cation ordering in MgAl2O4 spinel up to 1600 C from in situ neutron diffraction Data collected at IPNS, Argonne National Laboratory, T = 364 K on heating cycle, Mg.99Al2O4
Redfern, S. A. T.; Harrison, R. J.; O'Neill H St C; Wood, D. R. R.; American Mineralogist 84 (1999) 299–310; doi:

data_9002097
_publ_section_title
;Thermodynamics and kinetics of cation ordering in MgAl2O4 spinel up to 1600 C
 from in situ neutron diffraction Data collected at IPNS, Argonne National
 Laboratory, T = 364 K on heating cycle, Mg.99Al2O4
;
_journal_name_full               'American Mineralogist'
_journal_page_first              299
_journal_page_last               310
_journal_volume                  84
_journal_year                    1999
_chemical_formula_sum            'Al2 Mg O4'
_chemical_name_mineral           Spinel
_space_group_IT_number           227
_symmetry_space_group_name_Hall  '-F 4vw 2vw 3'
_symmetry_space_group_name_H-M   'F d -3 m :2'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            8
_cell_length_a                   8.09580
_cell_length_b                   8.09580
_cell_length_c                   8.09580
_cell_volume                     530.615
_database_code_amcsd             0002159
_diffrn_ambient_temperature      364
_exptl_crystal_density_diffrn    3.562
_cod_original_sg_symbol_H-M      'F d 3 m'
_cod_original_formula_sum        '(Mg Al2) O4'
_cod_database_code               9002097
Thermodynamics and kinetics of cation ordering in MgAl2O4 spinel up to 1600 C from in situ neutron diffraction Data collected at IPNS, Argonne National Laboratory, T = 374 K on heating cycle, Mg.99Al2O4
Redfern, S. A. T.; Harrison, R. J.; O'Neill H St C; Wood, D. R. R.; American Mineralogist 84 (1999) 299–310; doi:

data_9002098
_publ_section_title
;Thermodynamics and kinetics of cation ordering in MgAl2O4 spinel up to 1600 C
 from in situ neutron diffraction Data collected at IPNS, Argonne National
 Laboratory, T = 374 K on heating cycle, Mg.99Al2O4
;
_journal_name_full               'American Mineralogist'
_journal_page_first              299
_journal_page_last               310
_journal_volume                  84
_journal_year                    1999
_chemical_formula_sum            'Al2 Mg O4'
_chemical_name_mineral           Spinel
_space_group_IT_number           227
_symmetry_space_group_name_Hall  '-F 4vw 2vw 3'
_symmetry_space_group_name_H-M   'F d -3 m :2'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            8
_cell_length_a                   8.09613
_cell_length_b                   8.09613
_cell_length_c                   8.09613
_cell_volume                     530.680
_database_code_amcsd             0002160
_diffrn_ambient_temperature      374
_exptl_crystal_density_diffrn    3.561
_cod_original_sg_symbol_H-M      'F d 3 m'
_cod_original_formula_sum        '(Mg Al2) O4'
_cod_database_code               9002098
Thermodynamics and kinetics of cation ordering in MgAl2O4 spinel up to 1600 C from in situ neutron diffraction Data collected at IPNS, Argonne National Laboratory, T = 420 K on heating cycle, Mg.99Al2O4
Redfern, S. A. T.; Harrison, R. J.; O'Neill H St C; Wood, D. R. R.; American Mineralogist 84 (1999) 299–310; doi:

data_9002099
_publ_section_title
;Thermodynamics and kinetics of cation ordering in MgAl2O4 spinel up to 1600 C
 from in situ neutron diffraction Data collected at IPNS, Argonne National
 Laboratory, T = 420 K on heating cycle, Mg.99Al2O4
;
_journal_name_full               'American Mineralogist'
_journal_page_first              299
_journal_page_last               310
_journal_volume                  84
_journal_year                    1999
_chemical_formula_sum            'Al2 Mg O4'
_chemical_name_mineral           Spinel
_space_group_IT_number           227
_symmetry_space_group_name_Hall  '-F 4vw 2vw 3'
_symmetry_space_group_name_H-M   'F d -3 m :2'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            8
_cell_length_a                   8.09924
_cell_length_b                   8.09924
_cell_length_c                   8.09924
_cell_volume                     531.291
_database_code_amcsd             0002161
_diffrn_ambient_temperature      420
_exptl_crystal_density_diffrn    3.557
_cod_original_cell_volume        531.292
_cod_original_sg_symbol_H-M      'F d 3 m'
_cod_original_formula_sum        '(Mg Al2) O4'
_cod_database_code               9002099
Thermodynamics and kinetics of cation ordering in MgAl2O4 spinel up to 1600 C from in situ neutron diffraction Data collected at IPNS, Argonne National Laboratory, T = 502 K on heating cycle, Mg.99Al2O4
Redfern, S. A. T.; Harrison, R. J.; O'Neill H St C; Wood, D. R. R.; American Mineralogist 84 (1999) 299–310; doi:

data_9002100
_publ_section_title
;Thermodynamics and kinetics of cation ordering in MgAl2O4 spinel up to 1600 C
 from in situ neutron diffraction Data collected at IPNS, Argonne National
 Laboratory, T = 502 K on heating cycle, Mg.99Al2O4
;
_journal_name_full               'American Mineralogist'
_journal_page_first              299
_journal_page_last               310
_journal_volume                  84
_journal_year                    1999
_chemical_formula_sum            'Al2 Mg O4'
_chemical_name_mineral           Spinel
_space_group_IT_number           227
_symmetry_space_group_name_Hall  '-F 4vw 2vw 3'
_symmetry_space_group_name_H-M   'F d -3 m :2'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            8
_cell_length_a                   8.10384
_cell_length_b                   8.10384
_cell_length_c                   8.10384
_cell_volume                     532.197
_database_code_amcsd             0002162
_diffrn_ambient_temperature      502
_exptl_crystal_density_diffrn    3.551
_cod_original_sg_symbol_H-M      'F d 3 m'
_cod_original_formula_sum        '(Mg Al2) O4'
_cod_database_code               9002100
Thermodynamics and kinetics of cation ordering in MgAl2O4 spinel up to 1600 C from in situ neutron diffraction Data collected at IPNS, Argonne National Laboratory, T = 563 K on heating cycle, Mg.99Al2O4
Redfern, S. A. T.; Harrison, R. J.; O'Neill H St C; Wood, D. R. R.; American Mineralogist 84 (1999) 299–310; doi:

data_9002101
_publ_section_title
;Thermodynamics and kinetics of cation ordering in MgAl2O4 spinel up to 1600 C
 from in situ neutron diffraction Data collected at IPNS, Argonne National
 Laboratory, T = 563 K on heating cycle, Mg.99Al2O4
;
_journal_name_full               'American Mineralogist'
_journal_page_first              299
_journal_page_last               310
_journal_volume                  84
_journal_year                    1999
_chemical_formula_sum            'Al2 Mg O4'
_chemical_name_mineral           Spinel
_space_group_IT_number           227
_symmetry_space_group_name_Hall  '-F 4vw 2vw 3'
_symmetry_space_group_name_H-M   'F d -3 m :2'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            8
_cell_length_a                   8.10870
_cell_length_b                   8.10870
_cell_length_c                   8.10870
_cell_volume                     533.155
_database_code_amcsd             0002163
_diffrn_ambient_temperature      563
_exptl_crystal_density_diffrn    3.545
_cod_original_sg_symbol_H-M      'F d 3 m'
_cod_original_formula_sum        '(Mg Al2) O4'
_cod_database_code               9002101
Thermodynamics and kinetics of cation ordering in MgAl2O4 spinel up to 1600 C from in situ neutron diffraction Data collected at IPNS, Argonne National Laboratory, T = 636 K on heating cycle, Mg.99Al2O4
Redfern, S. A. T.; Harrison, R. J.; O'Neill H St C; Wood, D. R. R.; American Mineralogist 84 (1999) 299–310; doi:

data_9002102
_publ_section_title
;Thermodynamics and kinetics of cation ordering in MgAl2O4 spinel up to 1600 C
 from in situ neutron diffraction Data collected at IPNS, Argonne National
 Laboratory, T = 636 K on heating cycle, Mg.99Al2O4
;
_journal_name_full               'American Mineralogist'
_journal_page_first              299
_journal_page_last               310
_journal_volume                  84
_journal_year                    1999
_chemical_formula_sum            'Al2 Mg O4'
_chemical_name_mineral           Spinel
_space_group_IT_number           227
_symmetry_space_group_name_Hall  '-F 4vw 2vw 3'
_symmetry_space_group_name_H-M   'F d -3 m :2'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            8
_cell_length_a                   8.11359
_cell_length_b                   8.11359
_cell_length_c                   8.11359
_cell_volume                     534.120
_database_code_amcsd             0002164
_diffrn_ambient_temperature      636
_exptl_crystal_density_diffrn    3.538
_cod_original_sg_symbol_H-M      'F d 3 m'
_cod_original_formula_sum        '(Mg Al2) O4'
_cod_database_code               9002102
Thermodynamics and kinetics of cation ordering in MgAl2O4 spinel up to 1600 C from in situ neutron diffraction Data collected at IPNS, Argonne National Laboratory, T = 707 K on heating cycle, Mg.99Al2O4
Redfern, S. A. T.; Harrison, R. J.; O'Neill H St C; Wood, D. R. R.; American Mineralogist 84 (1999) 299–310; doi:

data_9002103
_publ_section_title
;Thermodynamics and kinetics of cation ordering in MgAl2O4 spinel up to 1600 C
 from in situ neutron diffraction Data collected at IPNS, Argonne National
 Laboratory, T = 707 K on heating cycle, Mg.99Al2O4
;
_journal_name_full               'American Mineralogist'
_journal_page_first              299
_journal_page_last               310
_journal_volume                  84
_journal_year                    1999
_chemical_formula_sum            'Al2 Mg O4'
_chemical_name_mineral           Spinel
_space_group_IT_number           227
_symmetry_space_group_name_Hall  '-F 4vw 2vw 3'
_symmetry_space_group_name_H-M   'F d -3 m :2'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            8
_cell_length_a                   8.11850
_cell_length_b                   8.11850
_cell_length_c                   8.11850
_cell_volume                     535.091
_database_code_amcsd             0002165
_diffrn_ambient_temperature      707
_exptl_crystal_density_diffrn    3.532
_cod_original_sg_symbol_H-M      'F d 3 m'
_cod_original_formula_sum        '(Mg Al2) O4'
_cod_database_code               9002103
Thermodynamics and kinetics of cation ordering in MgAl2O4 spinel up to 1600 C from in situ neutron diffraction Data collected at IPNS, Argonne National Laboratory, T = 778 K on heating cycle, Mg.99Al2O4
Redfern, S. A. T.; Harrison, R. J.; O'Neill H St C; Wood, D. R. R.; American Mineralogist 84 (1999) 299–310; doi:

data_9002104
_publ_section_title
;Thermodynamics and kinetics of cation ordering in MgAl2O4 spinel up to 1600 C
 from in situ neutron diffraction Data collected at IPNS, Argonne National
 Laboratory, T = 778 K on heating cycle, Mg.99Al2O4
;
_journal_name_full               'American Mineralogist'
_journal_page_first              299
_journal_page_last               310
_journal_volume                  84
_journal_year                    1999
_chemical_formula_sum            'Al2 Mg O4'
_chemical_name_mineral           Spinel
_space_group_IT_number           227
_symmetry_space_group_name_Hall  '-F 4vw 2vw 3'
_symmetry_space_group_name_H-M   'F d -3 m :2'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            8
_cell_length_a                   8.12333
_cell_length_b                   8.12333
_cell_length_c                   8.12333
_cell_volume                     536.046
_database_code_amcsd             0002166
_diffrn_ambient_temperature      778
_exptl_crystal_density_diffrn    3.526
_cod_original_sg_symbol_H-M      'F d 3 m'
_cod_original_formula_sum        '(Mg Al2) O4'
_cod_database_code               9002104
Thermodynamics and kinetics of cation ordering in MgAl2O4 spinel up to 1600 C from in situ neutron diffraction Data collected at IPNS, Argonne National Laboratory, T = 848 K on heating cycle, Mg.99Al2O4
Redfern, S. A. T.; Harrison, R. J.; O'Neill H St C; Wood, D. R. R.; American Mineralogist 84 (1999) 299–310; doi:

data_9002105
_publ_section_title
;Thermodynamics and kinetics of cation ordering in MgAl2O4 spinel up to 1600 C
 from in situ neutron diffraction Data collected at IPNS, Argonne National
 Laboratory, T = 848 K on heating cycle, Mg.99Al2O4
;
_journal_name_full               'American Mineralogist'
_journal_page_first              299
_journal_page_last               310
_journal_volume                  84
_journal_year                    1999
_chemical_formula_sum            'Al2 Mg O4'
_chemical_name_mineral           Spinel
_space_group_IT_number           227
_symmetry_space_group_name_Hall  '-F 4vw 2vw 3'
_symmetry_space_group_name_H-M   'F d -3 m :2'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            8
_cell_length_a                   8.12816
_cell_length_b                   8.12816
_cell_length_c                   8.12816
_cell_volume                     537.003
_database_code_amcsd             0002167
_diffrn_ambient_temperature      848
_exptl_crystal_density_diffrn    3.519
_cod_original_sg_symbol_H-M      'F d 3 m'
_cod_original_formula_sum        '(Mg Al2) O4'
_cod_database_code               9002105
Thermodynamics and kinetics of cation ordering in MgAl2O4 spinel up to 1600 C from in situ neutron diffraction Data collected at IPNS, Argonne National Laboratory, T = 916 K on heating cycle, Mg.99Al2O4
Redfern, S. A. T.; Harrison, R. J.; O'Neill H St C; Wood, D. R. R.; American Mineralogist 84 (1999) 299–310; doi:

data_9002106
_publ_section_title
;Thermodynamics and kinetics of cation ordering in MgAl2O4 spinel up to 1600 C
 from in situ neutron diffraction Data collected at IPNS, Argonne National
 Laboratory, T = 916 K on heating cycle, Mg.99Al2O4
;
_journal_name_full               'American Mineralogist'
_journal_page_first              299
_journal_page_last               310
_journal_volume                  84
_journal_year                    1999
_chemical_formula_sum            'Al2 Mg O4'
_chemical_name_mineral           Spinel
_space_group_IT_number           227
_symmetry_space_group_name_Hall  '-F 4vw 2vw 3'
_symmetry_space_group_name_H-M   'F d -3 m :2'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            8
_cell_length_a                   8.13321
_cell_length_b                   8.13321
_cell_length_c                   8.13321
_cell_volume                     538.005
_database_code_amcsd             0002168
_diffrn_ambient_temperature      916
_exptl_crystal_density_diffrn    3.513
_cod_original_sg_symbol_H-M      'F d 3 m'
_cod_original_formula_sum        '(Mg Al2) O4'
_cod_database_code               9002106
Thermodynamics and kinetics of cation ordering in MgAl2O4 spinel up to 1600 C from in situ neutron diffraction Data collected at IPNS, Argonne National Laboratory, T = 984 K on heating cycle, Mg.99Al2O4
Redfern, S. A. T.; Harrison, R. J.; O'Neill H St C; Wood, D. R. R.; American Mineralogist 84 (1999) 299–310; doi:

data_9002107
_publ_section_title
;Thermodynamics and kinetics of cation ordering in MgAl2O4 spinel up to 1600 C
 from in situ neutron diffraction Data collected at IPNS, Argonne National
 Laboratory, T = 984 K on heating cycle, Mg.99Al2O4
;
_journal_name_full               'American Mineralogist'
_journal_page_first              299
_journal_page_last               310
_journal_volume                  84
_journal_year                    1999
_chemical_formula_sum            'Al2 Mg O4'
_chemical_name_mineral           Spinel
_space_group_IT_number           227
_symmetry_space_group_name_Hall  '-F 4vw 2vw 3'
_symmetry_space_group_name_H-M   'F d -3 m :2'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            8
_cell_length_a                   8.13801
_cell_length_b                   8.13801
_cell_length_c                   8.13801
_cell_volume                     538.958
_database_code_amcsd             0002169
_diffrn_ambient_temperature      984
_exptl_crystal_density_diffrn    3.507
_cod_original_sg_symbol_H-M      'F d 3 m'
_cod_original_formula_sum        '(Mg Al2) O4'
_cod_database_code               9002107
Thermodynamics and kinetics of cation ordering in MgAl2O4 spinel up to 1600 C from in situ neutron diffraction Data collected at IPNS, Argonne National Laboratory, T = 1080 K on heating cycle, Mg.99Al2O4
Redfern, S. A. T.; Harrison, R. J.; O'Neill H St C; Wood, D. R. R.; American Mineralogist 84 (1999) 299–310; doi:

data_9002108
_publ_section_title
;Thermodynamics and kinetics of cation ordering in MgAl2O4 spinel up to 1600 C
 from in situ neutron diffraction Data collected at IPNS, Argonne National
 Laboratory, T = 1080 K on heating cycle, Mg.99Al2O4
;
_journal_name_full               'American Mineralogist'
_journal_page_first              299
_journal_page_last               310
_journal_volume                  84
_journal_year                    1999
_chemical_formula_sum            'Al2 Mg O4'
_chemical_name_mineral           Spinel
_space_group_IT_number           227
_symmetry_space_group_name_Hall  '-F 4vw 2vw 3'
_symmetry_space_group_name_H-M   'F d -3 m :2'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            8
_cell_length_a                   8.14282
_cell_length_b                   8.14282
_cell_length_c                   8.14282
_cell_volume                     539.914
_database_code_amcsd             0002170
_diffrn_ambient_temperature      1080
_exptl_crystal_density_diffrn    3.500
_cod_original_sg_symbol_H-M      'F d 3 m'
_cod_original_formula_sum        '(Mg Al2) O4'
_cod_database_code               9002108
Thermodynamics and kinetics of cation ordering in MgAl2O4 spinel up to 1600 C from in situ neutron diffraction Data collected at IPNS, Argonne National Laboratory, T = 1116 K on heating cycle, Mg.99Al2O4
Redfern, S. A. T.; Harrison, R. J.; O'Neill H St C; Wood, D. R. R.; American Mineralogist 84 (1999) 299–310; doi:

data_9002109
_publ_section_title
;Thermodynamics and kinetics of cation ordering in MgAl2O4 spinel up to 1600 C
 from in situ neutron diffraction Data collected at IPNS, Argonne National
 Laboratory, T = 1116 K on heating cycle, Mg.99Al2O4
;
_journal_name_full               'American Mineralogist'
_journal_page_first              299
_journal_page_last               310
_journal_volume                  84
_journal_year                    1999
_chemical_formula_sum            'Al2 Mg O4'
_chemical_name_mineral           Spinel
_space_group_IT_number           227
_symmetry_space_group_name_Hall  '-F 4vw 2vw 3'
_symmetry_space_group_name_H-M   'F d -3 m :2'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            8
_cell_length_a                   8.14757
_cell_length_b                   8.14757
_cell_length_c                   8.14757
_cell_volume                     540.859
_database_code_amcsd             0002171
_diffrn_ambient_temperature      1116
_exptl_crystal_density_diffrn    3.494
_cod_original_sg_symbol_H-M      'F d 3 m'
_cod_original_formula_sum        '(Mg Al2) O4'
_cod_database_code               9002109
Thermodynamics and kinetics of cation ordering in MgAl2O4 spinel up to 1600 C from in situ neutron diffraction Data collected at IPNS, Argonne National Laboratory, T = 1182 K on heating cycle, Mg.99Al2O4
Redfern, S. A. T.; Harrison, R. J.; O'Neill H St C; Wood, D. R. R.; American Mineralogist 84 (1999) 299–310; doi:

data_9002110
_publ_section_title
;Thermodynamics and kinetics of cation ordering in MgAl2O4 spinel up to 1600 C
 from in situ neutron diffraction Data collected at IPNS, Argonne National
 Laboratory, T = 1182 K on heating cycle, Mg.99Al2O4
;
_journal_name_full               'American Mineralogist'
_journal_page_first              299
_journal_page_last               310
_journal_volume                  84
_journal_year                    1999
_chemical_formula_sum            'Al2 Mg O4'
_chemical_name_mineral           Spinel
_space_group_IT_number           227
_symmetry_space_group_name_Hall  '-F 4vw 2vw 3'
_symmetry_space_group_name_H-M   'F d -3 m :2'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            8
_cell_length_a                   8.15239
_cell_length_b                   8.15239
_cell_length_c                   8.15239
_cell_volume                     541.820
_database_code_amcsd             0002172
_diffrn_ambient_temperature      1182
_exptl_crystal_density_diffrn    3.488
_cod_original_sg_symbol_H-M      'F d 3 m'
_cod_original_formula_sum        '(Mg Al2) O4'
_cod_database_code               9002110
Thermodynamics and kinetics of cation ordering in MgAl2O4 spinel up to 1600 C from in situ neutron diffraction Data collected at IPNS, Argonne National Laboratory, T = 1232 K on heating cycle, Mg.99Al2O4
Redfern, S. A. T.; Harrison, R. J.; O'Neill H St C; Wood, D. R. R.; American Mineralogist 84 (1999) 299–310; doi:

data_9002111
_publ_section_title
;Thermodynamics and kinetics of cation ordering in MgAl2O4 spinel up to 1600 C
 from in situ neutron diffraction Data collected at IPNS, Argonne National
 Laboratory, T = 1232 K on heating cycle, Mg.99Al2O4
;
_journal_name_full               'American Mineralogist'
_journal_page_first              299
_journal_page_last               310
_journal_volume                  84
_journal_year                    1999
_chemical_formula_sum            'Al2 Mg O4'
_chemical_name_mineral           Spinel
_space_group_IT_number           227
_symmetry_space_group_name_Hall  '-F 4vw 2vw 3'
_symmetry_space_group_name_H-M   'F d -3 m :2'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            8
_cell_length_a                   8.15738
_cell_length_b                   8.15738
_cell_length_c                   8.15738
_cell_volume                     542.815
_database_code_amcsd             0002173
_diffrn_ambient_temperature      1232
_exptl_crystal_density_diffrn    3.482
_cod_original_sg_symbol_H-M      'F d 3 m'
_cod_original_formula_sum        '(Mg Al2) O4'
_cod_database_code               9002111